LMucko/crystallography-open-database huggingface dataset:
Ternary halides of the A3 M X6 Typ II. The system Ag3-x Nax Y Cl6: Synthesis, structure ionic conductivity
Stenzel, F.; Meyer, G.; Zeitschrift fuer Anorganische und Allgemeine Chemie 619 (1993) 652–660; doi:10.1002/zaac.19936190406

data_1509588
_publ_section_title
;
 Ternary halides of the A3 M X6 Typ II. The system Ag3-x Nax Y Cl6:
 Synthesis, structure ionic conductivity
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              652
_journal_page_last               660
_journal_paper_doi               10.1002/zaac.19936190406
_journal_volume                  619
_journal_year                    1993
_chemical_formula_sum            'Ag1.3 Cl6 Na1.7 Y'
_chemical_name_systematic        '(Ag1.3 Na1.7) Y Cl6'
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   6.915
_cell_length_b                   6.915
_cell_length_c                   18.537
_cell_volume                     767.634
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            silver1-2_591.cif
_cod_data_source_block           Ag1.3Cl6Na1.7Y1
_cod_original_cell_volume        767.6345
_cod_original_formula_sum        'Ag1.3 Cl6 Na1.7 Y1'
_cod_database_code               1509588
The aluminium-rich corner of the Al-Mg-Ag phase diagram
Williams, B.E.; Journal of the Australian Institute of Metals 17 (1972) 171–174; doi:

data_1509589
_publ_section_title
;
 The aluminium-rich corner of the Al-Mg-Ag phase diagram
;
_journal_name_full
'Journal of the Australian Institute of Metals'
_journal_page_first              171
_journal_page_last               174
_journal_volume                  17
_journal_year                    1972
_chemical_formula_sum            'Ag1.334 Al0.666'
_chemical_name_systematic        '(Ag2 Al)0.66'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.88
_cell_length_b                   2.88
_cell_length_c                   4.58
_cell_volume                     32.899
_citation_journal_id_ASTM        JAMTAE
_cod_data_source_file            silver1-2_593.cif
_cod_data_source_block           Ag1.334Al0.666
_cod_original_cell_volume        32.89888
_cod_database_code               1509589
RMX compounds formed by alkaline earths, europium and ytterbium. IV: ternary phases with M = Ag and X =Si, Ge, Sn, Pb
Fornasini, M.L.; Merlo, F.; Pani, M.; Journal of Alloys Compd. 232 (1996) 289–295; doi:10.1016/0925-8388(95)01952-9

data_1509590
_publ_section_title
;
 RMX compounds formed by alkaline earths, europium and ytterbium. IV:
 ternary phases with M = Ag and X =Si, Ge, Sn, Pb
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              289
_journal_page_last               295
_journal_paper_doi               10.1016/0925-8388(95)01952-9
_journal_volume                  232
_journal_year                    1996
_chemical_formula_sum            'Ag1.346 Ba2 Si1.886'
_chemical_name_systematic        'Ba2 Ag1.346 Si1.886'
_space_group_IT_number           21
_symmetry_space_group_name_Hall  'C 2 2'
_symmetry_space_group_name_H-M   'C 2 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   8.612
_cell_length_b                   14.917
_cell_length_c                   19.633
_cell_volume                     2522.157
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            silver1-2_594.cif
_cod_data_source_block           Ag1.346Ba2Si1.886
_cod_database_code               1509590
Strukturverfeinerung des Freibergits
Kalbskopf, R.; Tschermaks Mineralogische und Petrographische Mitteilungen (-1978) 18 (1972) 147–155; doi:10.1007/BF01081799

data_1509591
_publ_section_title
;
 Strukturverfeinerung des Freibergits
;
_journal_name_full
;
Tschermaks Mineralogische und Petrographische Mitteilungen (-1978)
;
_journal_page_first              147
_journal_page_last               155
_journal_paper_doi               10.1007/BF01081799
_journal_volume                  18
_journal_year                    1972
_chemical_formula_sum            'Ag1.4 Cu10.6 S13 Sb4'
_chemical_name_systematic        'Ag1.4 Cu10.6 Sb4 S13'
_space_group_IT_number           217
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.503
_cell_length_b                   10.503
_cell_length_c                   10.503
_cell_volume                     1158.618
_citation_journal_id_ASTM        MPMTAG
_cod_data_source_file            silver1-2_595.cif
_cod_data_source_block           Ag1.4Cu10.6S13Sb4
_cod_database_code               1509591
Order-disorder transitions in the system Ag2-x Aux S (0<x<1)
Folmer, J.C.W.; Hofman, P.; Wiegers, G.A.; Journal of the Less-Common Metals 48 (1976) 251–268; doi:10.1016/0022-5088(76)90007-2

data_1509592
_publ_section_title
;
 Order-disorder transitions in the system Ag2-x Aux S (0<x<1)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              251
_journal_page_last               268
_journal_paper_doi               10.1016/0022-5088(76)90007-2
_journal_volume                  48
_journal_year                    1976
_chemical_formula_sum            'Ag1.43 Au0.66 S'
_space_group_IT_number           224
_symmetry_space_group_name_Hall  'P 4n 2 3 -1n'
_symmetry_space_group_name_H-M   'P n -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.95
_cell_length_b                   4.95
_cell_length_c                   4.95
_cell_volume                     121.287
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_596.cif
_cod_data_source_block           Ag1.43Au0.66S1
_cod_original_cell_volume        121.2874
_cod_original_sg_symbol_Hall     '-P 4bc 2bc 3 (x+1/4,y+1/4,z+1/4)'
_cod_original_formula_sum        'Ag1.43 Au0.66 S1'
_cod_database_code               1509592
The crystal structure of silver vanadate Ag(2-x) V4 O10 (x=0.57)
Belov, N.V.; Kuz'min, E.A.; Drozdov, Yu.N.; Doklady Akademii Nauk SSSR 210 (1973) 339–341; doi:

data_1509593
_publ_section_title
;
 The crystal structure of silver vanadate Ag(2-x) V4 O10 (x=0.57)
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              339
_journal_page_last               341
_journal_volume                  210
_journal_year                    1973
_chemical_formula_sum            'Ag1.43 O10 V4'
_chemical_name_systematic        'Ag1.43 V4 O10'
_space_group_IT_number           8
_symmetry_space_group_name_Hall  'B -2'
_symmetry_space_group_name_H-M   'B 1 1 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.4
_cell_formula_units_Z            2
_cell_length_a                   11.93
_cell_length_b                   8.81
_cell_length_c                   3.69
_cell_volume                     387.822
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            silver1-2_597.cif
_cod_data_source_block           Ag1.43O10V4
_cod_original_cell_volume        387.8217
_cod_original_sg_symbol_Hall     'C -2y (-x,z,y)'
_cod_database_code               1509593
Ternary gallides RE Agx Ga4-x (RE= La, Ce, Pr, Nd, Sm)
Grin', Yu.; Hiebl, K.; Eibler, R.; Rogl, P.; Journal of the Less-Common Metals 115 (1986) 367–372; doi:10.1016/0022-5088(86)90160-8

data_1509594
_publ_section_title
;
 Ternary gallides RE Agx Ga4-x (RE= La, Ce, Pr, Nd, Sm)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              367
_journal_page_last               372
_journal_paper_doi               10.1016/0022-5088(86)90160-8
_journal_volume                  115
_journal_year                    1986
_chemical_formula_sum            'Ag1.45 Ga6.55 Pr2'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.293
_cell_length_b                   4.293
_cell_length_c                   10.778
_cell_volume                     198.637
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_598.cif
_cod_data_source_block           Ag1.45Ga6.55Pr2
_cod_original_cell_volume        198.6369
_cod_database_code               1509594
Homologous silver bismuth chalcogenide halides (N,x)P.I. syntheses and crystal structures of the (0,1)P compound Ag Bi2 S2 Cl3 and of three members of the (1,x)P solid solution series Ag(x) Bi(4-2x) S(6-4x) Br(4x)
Ruck, M.; Soehnel, T.; Poudeu Poudeu, P.F.; Zeitschrift fuer Anorganische und Allgemeine Chemie 630 (2004) 1276–1285; doi:10.1002/zaac.200400131

data_1509595
_publ_section_title
;
 Homologous silver bismuth chalcogenide halides (N,x)P.I. syntheses and
 crystal structures of the (0,1)P compound Ag Bi2 S2 Cl3 and of three
 members of the (1,x)P solid solution series Ag(x) Bi(4-2x) S(6-4x) Br(4x)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              1276
_journal_page_last               1285
_journal_paper_doi               10.1002/zaac.200400131
_journal_volume                  630
_journal_year                    2004
_chemical_formula_sum            'Ag1.46 Bi2.54 Br2.91 S3.09'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.4
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   13.324
_cell_length_b                   4.093
_cell_length_c                   9.743
_cell_volume                     531.323
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            silver1-2_599.cif
_cod_data_source_block           Ag1.46Bi2.54Br2.91S3.09
_cod_original_cell_volume        531.3229
_cod_database_code               1509595
Die Kristallstrukturen von Zn9 Th, Cd2 Ca und (Ag, Mg)2 Ca
Nowotny, H.; Zeitschrift fuer Metallkunde 37 (1946) 31–34; doi:

data_1509596
_publ_section_title
;
 Die Kristallstrukturen von Zn9 Th, Cd2 Ca und (Ag, Mg)2 Ca
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              31
_journal_page_last               34
_journal_volume                  37
_journal_year                    1946
_chemical_formula_sum            'Ag1.48 Ca Mg0.52'
_chemical_name_systematic        '(Ag0.76 Mg0.24)2 Ca'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.843
_cell_length_b                   5.843
_cell_length_c                   9.5175
_cell_volume                     281.401
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            silver1-2_600.cif
_cod_data_source_block           Ag1.48Ca1Mg0.52
_cod_original_cell_volume        281.4008
_cod_original_formula_sum        'Ag1.48 Ca1 Mg0.52'
_cod_database_code               1509596
Preparation and characterization of the pseudobinary system Cu1-x Agx In Te2
Gopalam, B.S.V.; Krishna Rao, D.; Kasiviswanathan, S.; Journal of Materials Science 5 (1986) 912–914; doi:

data_1509597
_publ_section_title
;
 Preparation and characterization of the pseudobinary system Cu1-x Agx In
 Te2
;
_journal_name_full               'Journal of Materials Science'
_journal_page_first              912
_journal_page_last               914
_journal_volume                  5
_journal_year                    1986
_chemical_formula_sum            'Ag1.5 Cu0.5 In2 Te4'
_chemical_name_systematic        '(Ag1.5 Cu0.5) In2 Te4'
_space_group_IT_number           122
_symmetry_space_group_name_Hall  'I -4 2bw'
_symmetry_space_group_name_H-M   'I -4 2 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.3879
_cell_length_b                   6.3879
_cell_length_c                   12.5969
_cell_volume                     514.020
_citation_journal_id_ASTM        JMTSAS
_cod_data_source_file            silver1-2_601.cif
_cod_data_source_block           Ag1.5Cu0.5In2Te4
_cod_original_cell_volume        514.0198
_cod_database_code               1509597
Formation of an intermediate phase in eutectic Au - Ge and Ag - Ge systems under high pressure
Syono, Y.; Kusaba, K.; Kikegawa, T.; Iwasaki, H.; Fujinaga, Y.; Journal of the Less-Common Metals 170 (1991) 277–286; doi:10.1016/0022-5088(91)90329-3

data_1509598
_publ_section_title
;
 Formation of an intermediate phase in eutectic Au - Ge and Ag - Ge
 systems under high pressure
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              277
_journal_page_last               286
_journal_paper_doi               10.1016/0022-5088(91)90329-3
_journal_volume                  170
_journal_year                    1991
_chemical_formula_sum            'Ag1.5 Ge0.5'
_chemical_name_systematic        '(Ag3 Ge)0.5'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.86
_cell_length_b                   2.86
_cell_length_c                   4.666
_cell_volume                     33.053
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_602.cif
_cod_data_source_block           Ag1.5Ge0.5
_cod_original_cell_volume        33.05273
_cod_database_code               1509598
X-ray investigations of the Li - Ag - (Si, Ge) systems at 470 K
Bodak, O.I.; Kevorkov, D.G.; Pavlyuk, V.V.; Polish Journal of Chemistry 71 (1997) 712–715; doi:

data_1509599
_publ_section_title
;
 X-ray investigations of the Li - Ag - (Si, Ge) systems at 470 K
;
_journal_name_full               'Polish Journal of Chemistry'
_journal_page_first              712
_journal_page_last               715
_journal_volume                  71
_journal_year                    1997
_chemical_formula_sum            'Ag1.5 Ge Li1.5'
_chemical_name_systematic        '(Li3 Ag3 Ge2)0.5'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.045
_cell_length_b                   4.045
_cell_length_c                   4.045
_cell_volume                     66.184
_citation_journal_id_ASTM        PJCHDQ
_cod_data_source_file            silver1-2_603.cif
_cod_data_source_block           Ag1.5Ge1Li1.5
_cod_original_cell_volume        66.18439
_cod_original_formula_sum        'Ag1.5 Ge1 Li1.5'
_cod_database_code               1509599
The crystal structure and thermal stability of Ag In (Mo O4)2
Solodovnikov, S.F.; Klevtsov, P.V.; Perepelitsa, A.P.; Klevtsova, R.F.; Kristallografiya 29 (1984) 701–707; doi:

data_1509600
_publ_section_title
;
 The crystal structure and thermal stability of Ag In (Mo O4)2
;
_journal_name_full               Kristallografiya
_journal_page_first              701
_journal_page_last               707
_journal_volume                  29
_journal_year                    1984
_chemical_formula_sum            'Ag1.5 In1.5 Mo3 O12'
_chemical_name_systematic        'Ag (In0.75 Ag0.25)2 (Mo O4)3'
_space_group_IT_number           80
_symmetry_space_group_name_Hall  'I 4bw'
_symmetry_space_group_name_H-M   'I 41'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.998
_cell_length_b                   4.998
_cell_length_c                   36.725
_cell_volume                     917.391
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            silver1-2_604.cif
_cod_data_source_block           Ag1.5In1.5Mo3O12
_cod_original_cell_volume        917.3907
_cod_database_code               1509600
The thermodynamic and kinetic properties of silver intercalated niobium disulfide
Bouwmeester, H.J.M.; Solid State Ionics 16 (1985) 163–170; doi:

data_1509601
_publ_section_title
;
 The thermodynamic and kinetic properties of silver intercalated niobium
 disulfide
;
_journal_name_full               'Solid State Ionics'
_journal_page_first              163
_journal_page_last               170
_journal_volume                  16
_journal_year                    1985
_chemical_formula_sum            'Ag1.5 Nb6 S12'
_chemical_name_systematic        '(Ag Nb4 S8)1.5'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.3423
_cell_length_b                   3.3423
_cell_length_c                   39.35
_cell_volume                     380.685
_citation_journal_id_ASTM        SSIOD3
_cod_data_source_file            silver1-2_605.cif
_cod_data_source_block           Ag1.5Nb6S12
_cod_original_cell_volume        380.6854
_cod_database_code               1509601
_cod_duplicate_entry 1509082
The structure of the zeta phase in the silver-zinc system
Qurashi, M.M.; Edmunds, I.G.; Acta Crystallographica (1,1948-23,1967) 4 (1951) 417–427; doi:10.1107/S0365110X51001379

data_2310068
_publ_section_title
;
 The structure of the zeta phase in the silver-zinc system
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              417
_journal_page_last               427
_journal_paper_doi               10.1107/S0365110X51001379
_journal_volume                  4
_journal_year                    1951
_chemical_formula_sum            'Ag1.5 Zn1.5'
_space_group_IT_number           147
_symmetry_space_group_name_Hall  '-P 3'
_symmetry_space_group_name_H-M   'P -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   7.636
_cell_length_b                   7.636
_cell_length_c                   2.8197
_cell_volume                     142.385
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            silver1-2_606.cif
_cod_data_source_block           Ag1.5Zn1.5
_cod_original_cell_volume        142.3854
_cod_database_code               2310068
Order-disorder transitions in the system Ag2-x Aux S (0< x< 1)
Wiegers, G.A.; Hofman, P.; Folmer, J.C.W.; Journal of the Less-Common Metals 48 (1976) 251–268; doi:10.1016/0022-5088(76)90007-2

data_1509602
_publ_section_title
;
 Order-disorder transitions in the system Ag2-x Aux S (0< x< 1)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              251
_journal_page_last               268
_journal_paper_doi               10.1016/0022-5088(76)90007-2
_journal_volume                  48
_journal_year                    1976
_chemical_formula_sum            'Ag1.58 Au0.426 S'
_space_group_IT_number           224
_symmetry_space_group_name_Hall  'P 4n 2 3 -1n'
_symmetry_space_group_name_H-M   'P n -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.91
_cell_length_b                   4.91
_cell_length_c                   4.91
_cell_volume                     118.371
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_607.cif
_cod_data_source_block           Ag1.58Au0.426S1
_cod_original_cell_volume        118.3708
_cod_original_sg_symbol_Hall     '-P 4bc 2bc 3 (x+1/4,y+1/4,z+1/4)'
_cod_original_formula_sum        'Ag1.58 Au0.426 S1'
_cod_database_code               1509602
X-ray investigations of the Li - Ag - (Si, Ge) systems at 470 K
Pavlyuk, V.V.; Kevorkov, D.G.; Bodak, O.I.; Polish Journal of Chemistry 71 (1997) 712–715; doi:

data_1509603
_publ_section_title
;
 X-ray investigations of the Li - Ag - (Si, Ge) systems at 470 K
;
_journal_name_full               'Polish Journal of Chemistry'
_journal_page_first              712
_journal_page_last               715
_journal_volume                  71
_journal_year                    1997
_chemical_formula_sum            'Ag1.6 Li3.2 Si3.2'
_chemical_name_systematic        '(Li2 Ag Si2)1.6'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.05
_cell_length_b                   6.05
_cell_length_c                   6.05
_cell_volume                     221.445
_citation_journal_id_ASTM        PJCHDQ
_cod_data_source_file            silver1-2_608.cif
_cod_data_source_block           Ag1.6Li3.2Si3.2
_cod_original_cell_volume        221.4451
_cod_database_code               1509603
The effective valencies of transition metals in solid solutions in gold and silver alloys
Henderson, B.; Raynor, G.V.; Proceedings of the Royal Society of London, Series A: Mathematical and Physical Sciences (76,1906-) 267 (1962) 313–328; doi:10.1098/rspa.1962.0102

data_1509604
_publ_section_title
;
 The effective valencies of transition metals in solid solutions in gold
 and silver alloys
;
_journal_name_full
;
Proceedings of the Royal Society of London, Series A: Mathematical and
 Physical Sciences (76,1906-)
;
_journal_page_first              313
_journal_page_last               328
_journal_paper_doi               10.1098/rspa.1962.0102
_journal_volume                  267
_journal_year                    1962
_chemical_formula_sum            'Ag1.6 Mn0.1 Sn0.3'
_chemical_name_systematic        '(Ag16 Mn Sn3)0.1'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.9407
_cell_length_b                   2.9407
_cell_length_c                   4.7777
_cell_volume                     35.781
_citation_journal_id_ASTM        PRLAAZ
_cod_data_source_file            silver1-2_609.cif
_cod_data_source_block           Ag1.6Mn0.1Sn0.3
_cod_original_cell_volume        35.78088
_cod_database_code               1509604